Minerals Engineering 65 (2014) 61–73
Contents lists available at ScienceDirect
Minerals Engineering journal homepage: www.elsevier.com/locate/mineng
Surface characterisation, collector adsorption and ﬂotation response of enargite in a redox potential controlled environment Chris Plackowski a, Warren J. Bruckard b, Anh V. Nguyen a,⇑ a b
School of Chemical Engineering, The University of Queensland, Brisbane, Queensland 4072, Australia CSIRO Process Science and Engineering, Box 312, Clayton, Victoria, Australia
a r t i c l e
i n f o
Article history: Received 14 February 2014 Accepted 19 May 2014
Keywords: Arsenic Copper Xanthate Dithiophosphinate XPS Surface electrochemistry
a b s t r a c t We previously investigated oxidation of the surface of natural enargite (Cu3AsS4) under potentiostatic control and the formation of oxidation species at the mineral surface at selected applied potentials in the oxidative range. Here we further extended the research by incorporating ﬂotation collectors into the system. Electrochemical techniques, X-ray photoelectron spectroscopy (XPS) and microﬂotation in a redox potential controlled environment were applied to examine surface properties, collector adsorption and ﬂotation response of enargite in pH 10 solutions of sodium ethyl xanthate (SEX) and sodium dialkyl dithiophosphinate (3418A). The spectral details of XPS analysis of electrochemically treated enargite surfaces show signiﬁcant adsorption of SEX and 3418A collectors onto enargite at an applied voltage of +516 mV, but no adsorption of both collectors at 400 mV. The results of XPS analysis agree with the ﬂoatability of enargite determined by microﬂotation, showing that the ﬂotation recovery was highest at high oxidative potential (+516 mV), then decreased at low oxidative potential (+100 mV) and was very poor at 400 mV. These results conﬁrm that enargite ﬂoatability can be efﬁciently controlled electrochemically. Ó 2014 Elsevier Ltd. All rights reserved.
1. Introduction Enargite (Cu3AsS4) is an important mineral in the processing of copper ores due both to its value as a commercial source of copper, and the harmful impact of its arsenic content in terms of health, environmental, economic and ﬁnal product quality issues associated with its processing (Biswas and Davenport, 1994; Chatterjee et al., 1995; Cordova et al., 1997). A number of previous studies have investigated methods of separating arsenic and copper during the ﬂotation stage of mineral processing operations (Bruckard et al., 2010, 2007; Senior et al., 2006; Smith and Bruckard, 2007). The motivation for this work is the growing importance of ﬁnding an economic and effective means of reducing the arsenic levels in ﬂotation concentrates to acceptable levels. However, to date no effective ﬂotation method capable of selectivity for arsenic minerals in industrial applications has been developed. A recent review of the literature found that although some progress has been made in understanding the ﬂotation response of copper arsenic sulphides, fundamental knowledge of enargite surface chemistry must be further developed before the mechanisms that
⇑ Corresponding author. Tel.: +61 7 33653665; fax: +61 7 36654199. E-mail address: [email protected]
(A.V. Nguyen). http://dx.doi.org/10.1016/j.mineng.2014.05.013 0892-6875/Ó 2014 Elsevier Ltd. All rights reserved.
enable a successful separation by ﬂotation can be fully understood (Plackowski et al., 2012). Electrochemical techniques combined with surface analysis are useful methods to characterise a mineral surface and provide valuable information about its surface reactivity. Using this approach electrochemically induced surface oxidation of enargite by applied potentials of +869 mV at pH 10 and +610 mV at pH 4 has been investigated in a previous study (Plackowski et al., 2013b) (all voltages reported in this paper are relative to the standard hydrogen electrode (SHE) if not stated otherwise). Changes in surface morphology (roughness and distribution of surface products), hydrophobicity and surface speciation were found. Surface layer formations consisting of metal deﬁcient sulphide and elemental sulphur were identiﬁed, and a mechanism of Cu dissolution and diffusion-limited surface layer deposition was proposed. In this study only one applied potential of +869 mV at pH 10 was considered. In order to quantify surface chemical changes over a broad potential range, further work was completed (Plackowski et al., 2014). Five anodic potentials representing current peaks identiﬁed using cyclic voltammetry (+347, +516, +705, +869 and +1100 mV) were investigated to identify the chemical changes induced at the enargite surface in the oxidative range. These data can be used to identify potentials at which electrochemical reactions occur and, in combination with thermodynamic data, reaction mechanisms
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
proposed to be responsible for the chemical changes at the surface have been derived (Guo and Yen, 2008). Characterisation of the electrochemically oxidised surface using XPS provided partial conﬁrmation of these mechanisms but also revealed signiﬁcant differences in speciation, allowing alternative mechanisms to be formulated in combination with thermodynamic data (Plackowski et al., 2014). These previous studies considered a simple system where enargite is electrochemically oxidised in buffer solution with no other reagents present. To further develop our understanding of the ﬂotation response of enargite as a function of pulp potential additional complexity is required. In this paper XPS is used to examine the enargite surface and identify the surface chemical species present after treatment at oxidising and reducing potentials (+516 and 400 mV, respectively) in the presence of ﬂotation collector. Two commonly used collectors for sulphide minerals, namely sodium ethyl xanthate (SEX) and sodium dialkyl dithiophosphinate (DTPI), were chosen for this study. The ﬂotation response was investigated using the UCT microﬂotation cell as described by Bradshaw and O’Connor (1996). This was done to determine if there would be a difference in the ﬂotation response of enargite after conditioning in the presence of ﬂotation collector at pulp potentials equivalent to the electrochemically applied oxidising and reducing potentials used for the XPS work. The aim of this research work was to determine what differences exist in collector adsorption after treatment at these applied potentials, and if there is a correlation with the ﬂotation recovery of enargite in a simple single mineral microﬂotation system.
2. Experimental 2.1. Materials A high purity sample of natural enargite (Cu3AsS4) sourced from Wright’s Rock Shop (USA) was used for the experimental work. Initial characterisation was carried out by X-ray diffraction for determining its crystal structure and identifying the mineral phases present. Enargite was the predominant phase determined with no other signiﬁcant phases detected. Its chemical composition was conﬁrmed by XPS. A resin mounted thin polished section with the mineral exposed on both sides was prepared for the electrochemical work, and mounted on a fabricated PVC sample holder to facilitate preparation, handling and the experimental techniques. A pH 10.0 buffer solution (0.05 M) was prepared for the electrochemical work using di-sodium tetraborate decahydrate (Scharlau Chemie S.A., Spain, AR grade) and sodium hydroxide (Sigma–Aldrich, Australia, technical grade). Water freshly puriﬁed using a reverse osmosis RIO’s unit and an Ultrapure Academic Milli-Q system (Millipore, USA) was used in the experiments. The Milli-Q water had a speciﬁc resistance of 18.2 MX cm1. Collector solutions were prepared using pH 10 buffer as the base solution, to which SEX (Flottec, USA, commercial grade) and DTPI (Aerophine 3418A promoter, Cytec, USA) solutions were added to give the ﬁnal concentration of collector in solution required for the CV (cyclic voltammetry) and XPS studies. SEX was supplied in solid crystalline form, while DTPI was supplied as a 50 vol% solution made up with water. For the microﬂotation tests 0.1 M sodium hydroxide solution (Chem Supply, Australia, analytical reagent) and 0.1 M nitric acid solution (Ajax Finechem Pty Ltd, analytical reagent) were used for pH control, while sodium dithionite (Na2S2O4, Sigma Aldrich, technical grade) and sodium hypochlorite (NaOCl, APS Finechem, Australia, technical grade) solutions (2.5% w/v) were used to set and control the pulp potential.
2.2. Sample preparation The freshly polished mineral surface was prepared for XPS by electrochemical conditioning in a pH 10.0 buffer solution at selected potentials using an Asylum AFM electrochemical cell (Asylum, Santa Barbara, USA) and a Gamry Reference 600 potentiostat (Gamry, Warminster, USA). The solution consisted of either buffer alone or buffer containing selected concentrations of ﬂotation collector, depending on the test requirements. The potentiostat working electrode cable was connected to the enargite working electrode (resin mounted polished sample) by an insulated copper wire attached to its lower surface using silver epoxy (ITW Chemtronics, USA) to ensure good electrical contact, while a platinum wire was used as the counter electrode. A Ag/ AgCl 3 M KCl microelectrode (Microelectrodes Inc., USA) was used as the reference electrode. Prior to each measurement any pre-existing surface oxidation was removed by machine polishing with 9, 3 and 1 micron diamond suspensions (Dia-duo, Struers Australia) in sequence to ensure a fresh surface was exposed. The surface was then washed with ethanol (AR grade) and dried with high purity compressed nitrogen, and immediately transferred to the electrochemical cell. The reference and counter electrodes were then attached to the cell, the enargite surface covered with buffer solution and the oxidising potential initiated. To ensure all collector residue was removed from the mineral surface after each test, CV measurements were conducted after polishing to check that the response of the surface was the same as for a known clean enargite surface. Where the voltammogram did not match the clean surface, polishing and the CV measurement was repeated until no evidence of variation from the clean surface due to the presence of collector was found. Surface conditioning was performed as a single-step experiment using the chronoamperometry (CA) technique where the desired potential was applied for 10 min at room temperature (25 °C). The conditioning potentials were chosen based on the work of Senior et al. (2006) and Guo and Yen (2005) which investigated the effects of pulp potential on the ﬂotation response of enargite. These studies revealed the existence of a threshold potential range over which enargite undergoes a transition from non-ﬂoating to ﬂoating as the potential increases. Guo and Yen (2005) found this range to be about 150 to +200 mV for synthetic enargite at pH 10 in potassium amyl xanthate (PAX) solution, while Senior et al. (2006) found the transition occurred over the range 100 to +100 mV for natural enargite at pH 11 in the presence of potassium ethyl xanthate (KEX). To ensure conditioning was performed outside the transition potential range, potentials of 400 and +516 mV were selected. These potentials were chosen with reference to previous CV results which identiﬁed an oxidative current peak at +516 mV and a reductive peak at 400 mV (Plackowski et al., 2014). In addition these values were also considered sufﬁciently distant from the transition potential range identiﬁed by Senior et al. (2006) as between about 150 and 50 mV, below which enargite was found to be non-ﬂoatable and above which it was strongly ﬂoatable. Comparative testing was also carried out at approximately +100 mV to evaluate recovery within the transition potential range. 2.3. Electrochemistry To provide a baseline reference curve for enargite without collector, CV was performed with a freshly polished enargite sample in a pH 10.0 buffer solution using the Asylum AFM electrochemical cell and the Gamry Reference 600 potentiostat. The connections and electrodes are described in the section. All voltages have been
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
converted and reported relative to SHE (standard hydrogen electrode) as noted earlier. In preparation for a measurement, the sample was polished, washed with ethanol, dried with high purity N2 and quickly transferred to the electrochemical cell. The reference and counter electrodes were attached to the cell, the enargite surface covered with the required buffer solution (with or without collector) and the measurement initiated. All measurements were initiated in the positive potential direction and conducted at a scan rate of 1 mV/s: all CV curves were started from a potential of 0 mV at a sweep rate of 1 mV/s in the positive sweep direction, switched to the cathodic scan direction at 1100 mV, then switched back to the anodic direction at 690 mV and terminated at 0 mV. Deoxygenation of the buffer solution and electrochemical cell was not necessary (Plackowski et al., 2014). Surface preparation for XPS was carried out using the CA technique performed as a single-step experiment at the selected conditioning potentials of either 400 or +516 mV. Using this method the selected potential is applied to the enargite working electrode and the resulting current measured over a pre-determined period of time. In the present work the conditioning potential was applied for 600 s to a freshly polished enargite surface immersed in a quiescent pH 10 buffer solution with or without collector as required. The conditioning potentials were selected based on the proposed threshold potential for enargite ﬂotation as discussed earlier. 2.4. X-ray photoelectron spectroscopy XPS measurements of the enargite surface after treatment using the experimental procedures described above were carried out to identify the chemical species formed at oxidising or reducing potentials of +516 and 400 mV, respectively. Data was acquired using a Kratos Axis ULTRA X-ray Photoelectron Spectrometer incorporating a 165 mm hemispherical electron energy analyzer. The incident radiation was monochromatic Al Ka X-rays (1486.6 eV) at 150 W (15 kV, 15 mA). The instrument work function was calibrated to give a binding energy (BE) of 83.96 eV for the Au 4f7/2 line for metallic gold and the spectrometer dispersion was adjusted to give a BE of 932.62 eV for the Cu 2p3/2 line of metallic copper. Detection limits ranged from 0.1 to 0.5 atomic percent depending on the element. The Kratos charge neutralizer system was used on all specimens. Survey (wide) scans were taken with an analysis area of 300 700 lm at an analyzer pass energy of 160 eV. Multiplex (narrow) high resolution scans were carried out with an analysis area of 300 700 lm and an analyzer pass energy of 20 eV. Survey scans were carried out over a 1200–0 eV binding energy range with 1.0 eV steps and a dwell time of 100 ms. Narrow high-resolution scans were run with 0.05 eV steps and 250 ms dwell time. Base pressure in the sample analysis chamber (SAC) was 1.0 109 torr and during sample analysis it was 1.0 108 torr. Spectra have been charge corrected using the main line of the carbon 1s spectrum photoelectron peak (adventitious carbon) as an internal reference to account for sample charging, with an assigned BE of 284.8 eV, and were analysed using the CasaXPS software (version 2.3.14). The oxidised enargite specimen was secured to a metal stub with conductive tape in preparation for the measurement, which was then attached to the sample holder and inserted into the loading chamber. Sample cooling was used for all measurements. The sample holder was pre-cooled to liquid nitrogen temperatures by a cold probe before evacuation of the XPS instrument loading chamber. This procedure is designed to preserve volatile species on the specimen surface, which have been demonstrated to be unstable without cooling (Plackowski et al., 2013a). During initial cooling the chamber was continuously ﬂushed with high purity dry nitrogen to remove moisture and oxygen. Once a temperature
of 100 °C was reached the chamber was sealed and evacuation commenced. Once the required vacuum was reached the specimen was then transferred to the SAC and attached to the pre-cooled sample stage, where it was maintained at 135 °C throughout the measurement. A single survey scan was ﬁrst completed to identify surface elemental composition and then multiplex high resolution scans of each elemental region were completed. From these spectral distributions, the relative elemental concentrations, oxidation state and chemical bonding associations were determined. Relative elemental atomic concentrations were determined by peak ﬁtting using the CASA XPS software package and the Kratos library of sensitivity factors. XPS data for the Cu 2p, O 1s, C 1s, S 2p and As 3d regions was ﬁtted using Shirley background subtraction and Gaussian–Lorentzian peak proﬁles. The XPS analysis of oxidised enargite has been shown to be dependent on the temperature at which it is carried out (Fantauzzi et al., 2006), as is the general case for other sulphides (Hampton et al., 2011; Wittstock et al., 1996). At ambient temperature, the ultrahigh vacuum required during analysis (1.0 108 torr) creates an environment where elemental sulphur formed on the surface is unstable and evaporates. In addition, it has been reported that Cu(II) species, in particular Cu(OH)2, undergo a combination of vacuum and thermal dehydration and decomposition to CuO at ambient temperature (Skinner et al., 1996), typically found to be about 30 °C in the XPS sample analysis chamber. This effect can be controlled by pre-cooling (below 130 °C) the sample before evacuation thereby limiting evaporation of sulphur and decomposition of Cu(OH)2 and other unstable compounds on the surface. When cooling is not used, elemental sulphur present on the surface quickly evaporates and so is lost and not detected, while other compounds undergo degradation. The effects of XPS analysis on the surface species present on oxidised enargite was investigated in a previous study (Plackowski et al., 2013a), and similar behaviour as seen for other sulphides was demonstrated. For this reason the sample was cooled in the loading chamber using a liquid nitrogen system to below 130 °C prior to evacuation. After transfer it was maintained at that temperature in the SAC. 2.5. Microﬂotation Microﬂotation tests were conducted to conﬁrm the effects of conditioning at different redox potentials in the presence of collector on the ﬂotation recovery of enargite. The UCT microﬂotation cell as described by Bradshaw and O’Connor (1996) was used for this purpose and is shown diagrammatically in Fig. 1. The mineral used was natural enargite as described in Section 3.1, in the size range of 53–106 lm. Following the method described by Bradshaw and O’Connor (1996), for each test 2 g of enargite was added to 50 mL of de-ionised water and treated in an ultrasonic bath for 10 min to remove any ﬁne particles and oxidised surface material, then washed and ﬁltered. The ﬂotation solution was prepared separately with de-ionised water, the pH was set as required using sodium hydroxide and nitric acid solutions as needed, while Eh was set using sodium hypochlorite solution or sodium dithionite solution. Once the desired values were reached the solution was transferred to the ﬂotation cell, and the pH and Eh checked and adjusted as required. The mineral was then placed in the ﬂotation cell and the peristaltic pump set to 130 rpm (ﬂow rate 1.8 L/min), and the pH and Eh checked and adjusted again if required. The desired ﬂotation collector was then added and the pulp conditioned for 5 min. Throughout conditioning pH and Eh were monitored and adjusted if needed. The positive and transition potentials (+500 and +100 mV, respectively) were found to be stable throughout
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
Fig. 1. Schematic of the UCT microﬂotation apparatus (after Bradshaw and O’Connor, 1996) used in this study. 0.3
Current Density (mA/cm2)
conditioning. However, reagent addition was required to maintain the cathodic potential (400 mV). Nitrogen was used as the ﬂotation gas, and at the commencement of ﬂotation the syringe was inserted at the base of the cell with a pre-set ﬂow rate of 8 mL/min. After a ﬂotation time of 1 min, the syringe was removed and the recovered enargite ﬁltered and weighed. Recovery was determined as the mass fraction of enargite reporting to the concentrate.
0.2 0.1 0.0 -0.1 -0.2
3. Results and discussion -0.3 -800
3.1. Cyclic voltammetry
Current Density (mA/cm2 )
0.4 0.3 0.2 0.1 0.0 -0.1 -0.2
Applied Potential (mV SHE)
Previous investigations (Plackowski et al., 2013b) have examined the current response to applied potential of natural enargite in pH 10 buffer solution alone and the resulting CV curve for a freshly polished natural enargite surface is shown in Fig. 2. These results support the work of Guo and Yen (2006, 2008) who compared natural and synthetic enargite at pH 10, and Velasquez et al. (2000) and Cordova et al. (1997), who investigated natural enargite at pH 9.2. Those differences that can be seen between the present work and the published data were considered the result of variations in mineral composition, such as the type and concentrations of impurities present, sample preparation, and experimental method. In the anodic portion of the scan ﬁve current peaks were observed at potentials of +347, +516, +705, +869 and +1100 mV,
Applied Potential (mV SHE) Fig. 2. Typical cyclic polarisation curve for natural enargite at pH 10 obtained using a scan rate of 1 mV/s (Plackowski et al., 2013b).
Fig. 3. Reactivity of the enargite surface in the presence of 106, 105, 104 and 103 M SEX in pH 10 buffer solutions.
labelled as peaks 1–5 in Fig. 1, respectively. The peak at +516 mV is not clearly evident in the ﬁgure, but a local current maximum can be seen at this potential in the numerical data. These potentials are similar to those found by Guo and Yen (2008), who reported ﬁve anodic CV peaks at +228, +548, +728, +826 and +1074 mV. In the cathodic sweep current peaks are seen at 100 mV, 100 mV and 400 mV (numbered 6–8, respectively). In addition a peak is present at about 790 mV in the oxidative range on the return sweep from 1100 mV. Such a peak was not present in the data of Guo and Yen (2008). One possible explanation for its presence is that it represents the continuation of a reaction process ﬁrst occurring at about 800 mV during the anodic scan in the forward sweep direction. Peak 3 represents the highest current density observed, the enargite surface has greater reactivity at this potential and this reaction does not reach equilibrium, even at the low sweep rate of 1 mV/s used. Changes in the surface reactivity were also investigated using CV, where enargite was immersed in the same pH 10 buffer solution, containing different concentrations of ﬂotation collectors. Shown in Fig. 3 are the cyclic voltammograms for enargite in the presence of SEX at different concentrations. The effect of surface potential on the contact angle of the mineral surface in a 7 104 M PAX solution at pH 7 and 10 was investigate by Guo and Yen (2002). The relatively high concentration was chosen to ensure a constant xanthate concentration during the measurement. The oxidation of xanthate to form dixanthogen during anodic polarisation was observed as an emulsion
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
surrounding the mineral surface. Hexane extracts of this solution were identiﬁed as dixanthogen using UV spectroscopy. The effect of PAX on the cyclic polarisation of enargite was also investigated by Guo and Yen (2006), where the effects of PAX concentrations of 0 and 104 M on the current density of enargite polarisation at pH 10 were compared. It was concluded that the PAX passivated the enargite surface at about 80 mV as a result of dixanthogen formation. Surface passivation during anodic polarisation in the presence of increasing concentrations of xanthate is supported by Guo (2004) who investigated the effects of increasing PAX concentration. In addition, cyclic polarisation of natural enargite in pH 10 buffer solution revealed ﬁve anodic current peaks at similar potentials to those shown in Fig. 2. Guo (2004) reported that increasing PAX concentration from 105 to 104 M caused the shift of peaks 1 and 3 to a higher potential while the current density of peaks 1 and 2 decreased. At 103 M xanthate concentration, peaks 1 and 2 were no longer present, and a new peak appeared in their place, representing the oxidation of xanthate to dixanthogen. Bagci et al. (2007) attribute a similar peak observed in a chalcopyrite and sodium isopropyl xanthate system to the adsorption of xanthate as CuX. Comparing the voltammograms of different xanthate concentrations in Fig. 3 it can be seen that the current density of peak 1 diminishes with increasing ‘concentration and a peak at low positive potential is present at a concentration of 103 M, suggestive of dixanthogen formation. Peak 3 is also shifted to a higher potential as a consequence of surface passivation by a hydrophobic dixanthogen layer, which prevents oxidation of the surface at lower anodic potentials. Although the interaction of DTPI collectors with sulphide minerals has been well studied in the literature (Bagci et al., 2007; Güler et al., 2006; Pecina et al., 2006), these works have focussed on the more common base metal and iron sulphides such as chalcopyrite, pyrite and galena. Limited information is available about the interaction of DTPIs with arsenic-bearing sulphides, of which enargite and tennantite (Cu12As4S13) are the most signiﬁcant in copper ore bodies (Petrus et al., 2011a). Of these two minerals, the adsorption of the related dithiophosphate (DTP) collector onto tennantite has been investigated (Petrus et al., 2011a,b), and the ﬂotation response of enargite with several collectors, including isopropyl xanthate and diisobutyl dithiophosphate, at pH 10.5, has been studied using a modiﬁed Hallimond tube (Castro et al., 2003). Fornasiero and co-workers (Fornasiero et al., 2001) studied the effects of selective oxidation or dissolution on the separation of enargite and tennantite from non-arsenic copper sulphides using diethyl dithiophosphate collector. Smith and Bruckard (2007) used sodium isobutyl xanthate and a dithiophosphate (AP 208) in their study of tennantite separation, while Senior et al. (2006) conducted single mineral studies of enargite using KEX collector. However
apart from pulp potential measurements these studies did not involve any investigation of the speciﬁc effects of these collectors on the electrochemical response of these systems. In this study sodium dialkyl dithiophosphinate (Aerophine 3418A promoter) was chosen for investigation as it is reported to be a strong collector for sulphides and selective against iron sulphide minerals. Electrochemical investigations show the effect of DTPI concentration on the cyclic polarisation of natural enargite at pH 10, as shown in Fig. 4. This outcome is similar to that seen with chalcopyrite (Güler et al., 2004) over a range of DTPI concentrations, although the voltammograms in this work are ﬁrst cycle, rather than ﬁfth cycle as used by Güler et al. (2004) hence the current peaks are more pronounced. Current density decreases proportionally with increasing DTPI concentration, which can be interpreted as indicative of the formation of a passivating layer on the mineral surface. This layer inhibits access of the surrounding solution to the surface, limiting redox activity and the formation of current density peaks in the cyclic voltammogram. 3.2. Surface composition of unoxidised (natural) enargite The composition of the natural enargite used for this study has been characterised using XPS, and the complete results are available in previously publications (Plackowski et al., 2014, 2013b). The complete XPS data is included in Table 1 for comparison with enargite used in the experimental studies. Characteristic photoelectron peaks were detected for copper, arsenic and sulphur, as well as for oxygen and carbon. The relative atomic concentrations of all elements differed only slightly with respect to the stoichiometric formula of enargite, i.e. Cu3AsS4, with concentrations of Cu 2p 27.1%, As 3d 12.3% and S 2p 35.9% detected. In previous work (Plackowski et al., 2014) thermodynamic data and XPS results, combined with other published work (Guo and Yen, 2008), were used as the basis for formulating new reaction mechanisms for oxidation of enargite by applied anodic potential. The reaction mechanism corresponding to an applied potential of +516 mV using natural enargite at pH 10 without collector is presented as follows (Plackowski et al., 2014):
Cu3x AsS4 þ ð14 2xÞOH ¼ ð3 xÞCu2þ þ ð6 2xÞOH 2 þ AsO3 4 þ 4Sn þ 4H2 O þ ð3 2xÞe
ð1Þ Plackowski et al. (2013b) also considered the cathodic scan returning from high applied potential (peaks 6–8 in Fig. 2), where the current peaks result from the reduction of copper hydroxide (peak 7 in Fig. 2) and elemental sulphur and polysulﬁde ions (peak 8, 400 mV). The reduction reactions can be presented as follows:
2CuðOHÞ2 þ 2e ¼ Cu2 O þ 2OH þ 2H2 O EðSHEÞ ¼ 95 mV
Current Density (mA/cm2)
Table 1 Binding energies, full width half-maxima (FWHM) and atomic concentrations (Atom%) of the elements identiﬁed on the freshly fractured enargite surface.
0.1 0.0 -0.1 -0.2 -0.3 -800
Applied Potential (mV SHE) Fig. 4. Reactivity of the enargite surface in the presence of 106, 105, 104, 103 and 102 M DTPI collector in pH 10 buffer solutions.
Cu 2p3/2 Cu 2p1/2 O 1s C 1s CAC ref S 2p3/2 S 2p1/2 As 3d5/2 (surface) As 3d3/2 (surface) As 3d5/2 (bulk) As 3d3/2 (bulk)
932.0 951.9 529.5 284.8 161.8 163.0 42.2 42.9 43.2 43.9
1.1 1.7 0.9 1.5 0.7 0.8 0.8 0.8 0.6 0.6
18.9 8.2 3.2 21.6 23.4 12.5 2.6 1.7 4.8 3.2
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
2S0 þ 2e ¼ S2 2 EðSHEÞ ¼ 670 mV
2 S2 EðSHEÞ ¼ 720 mV 2 þ 2e ¼ 2S
At low potential the reduction decomposition of enargite must also be considered, and includes arsenic sulphide and copper sulphide among its products as shown below:
2Cu3 AsS4 þ 6H2 O þ 6e ¼ As2 S2 þ 3Cu2 S þ 2H2 S þ 6OH
These mechanisms are useful to give an indication of the nature of the chemical species which may be present on the enargite surface as a result of electrochemical oxidation, thus providing a baseline reference for further studies. In this work XPS was used to investigate the enargite surface after application of an oxidising or reducing potential in the presence of a ﬂotation collector. The principal purpose was to identify whether the collector was present on the surface or not, and secondary to this, to identify the chemical species present. This information may then be useful to suggest the type of adsorption mechanism responsible for any surface layer formation. 3.3. Enargite in the presence of xanthate collector Changes in the elemental species detected on the surface of enargite at oxidising and reducing potentials in the presence of sodium ethyl xanthate were investigated by XPS to identify which species are present after treatment and to compare with untreated enargite. Analysis of the crystalline xanthate used to prepare the experimental solutions revealed the presence of Na 1s, O 1s, C 1s and S 2p species in accord with the chemical formula of sodium ethyl xanthate, CH3CH2OCS2Na, and the binding energies for each species are shown in Table 2. Fig. 5 shows the XPS photoelectron spectra recorded from enargite after conditioning for 10 min at +516 mV in SEX solution, while the binding energies are included in Table 3. In this enargite sample the O 1s spectrum shows the presence of an additional species at about 529.6 eV which was identiﬁed as antimony (Sb 3d5/2) and conﬁrmed by the presence of a corresponding Sb 3d3/2 peak at the correct area ratio and peak separation of 9.34 eV. It represents a minor contaminant at a concentration of about 0.3 atom%, and is present in other results shown below although for clarity has been omitted from the tables. Adsorption of xanthate on sulphide surfaces was investigated by Ranta et al. (1981) using XPS to determine the binding energies of C, O and S of KEX on synthetic thin sulphide layers. They report a S 2p BE of 163.7 eV for bulk KEX, although it appears insufﬁcient resolution was obtained to isolate the S 2p3/2 component, which makes comparison with the present results difﬁcult. In our work
Table 2 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed in crystalline SEX at 130 °C.
Na 1s O 1s O 1s OACAS C 1s CAC ref C 1s CACOO CAO CAS COO S 2p3/2 CS2 S 2p1/2 CS2 S 2p3/2 SO4 S 2p1/2 SO4
1071.6 531.5 533.2 284.8 285.4 286.2 287.5 288.5 162.0 163.2 168.2 169.4
1.3 1.4 1.3 1.0 0.9 1.0 0.9 1.0 0.9 0.9 0.9 0.9
15.9 6.5 9.2 20.4 1.8 11.0 9.4 1.8 10.8 5.4 0.4 0.2
S 2p3/2, 1/2 BEs of 162.0 and 163.2 eV were found for crystalline sodium ethyl xanthate. A BE range between 162.1 and 162.6 eV was reported by Ranta et al. (1981) for adsorbed xanthate, which is signiﬁcantly lower than the S 2p3/2 BE of 163.1 eV in this work. Such a comparison is useful to show the expected BE shift of the S 2p component between the bulk and adsorbed xanthate. Differences in S 2p BEs between SEX and KEX are shown to exist and, combined with the different substrates onto which they were adsorbed (Ranta et al., 1981) used a copper sheet with a thin layer of copper sulphide), direct comparison of these different systems is difﬁcult. According to Ranta et al. (1981), the C 1s spectra can be used to determine ethyl xanthate adsorption by the presence of a peak additional to the adventitious carbon peak (284.8 eV in the present work) between 286.3 and 286.5 eV, which compares well with our work where a second peak exists at 286.4 eV. Mielczarski (1987) also found a C 1s peak at about 286.5 eV after treatment of chalcocite with KEX, attributed to the CAOAC group in xanthate. The carbon atom in the CH3 group is characterised by a peak at about 284.9 eV and cannot be distinguished from hydrocarbon contamination, although it accounts for the signiﬁcant increase in this component compared to the fresh enargite surface (21.6– 30.1%). Considering the O 1s spectra, Ranta et al. (1981) report the presence of a new component at 532.9 eV after xanthate adsorption which they conclude indicates the presence of collector. Mielczarski (1987) reports an increase in the contribution of the O 1s component at 533.0 eV, which is due to oxygen from the xanthate. This is in good agreement with the O 1s peak detected at 533.4 eV in this work. Thus a comparison of the results from enargite conditioned at +516 mV to the fresh enargite surface reveals that clear differences in the S 2p, C 1s and O 1s spectra exist, which can be attributed to the presence of xanthate on the surface after conditioning. Regarding the nature of the surface xanthate species, the XPS results suggest the adsorption products detected on the enargite surface are more likely to be in the form of dixanthogen rather than copper xanthate, which in another study has been reported as the only adsorption product (Valli and Persson, 1994). Evidence for this contention is provided by the absence of any change in the Cu 2p spectrum, both in terms of BE and number of Cu species present, while the decrease in relative proportion of Cu can be interpreted as partial passivation of the surface by the formation of an incomplete xanthate surface layer. According to Mielczarski et al. (1996) while dixanthogen is often assumed to be the surface product, no consensus exists as to whether it and copper xanthate are formed concurrently or sequentially, and if so which is the ﬁrst to form. The XPS photoelectron spectra obtained after conditioning at 400 mV are shown in Fig. 6 and the associated binding energies in Table 4. After conditioning of enargite at 400 mV in the presence of sodium ethyl xanthate, XPS analysis shows the surface has undergone some changes, with additional O 1s and C 1s species present when compared to a clean surface. However only one S 2p species exists, and along with Cu 2p and As 3d peaks their BE’s remain unchanged compared to the fresh enargite surface. The presence of Cu 2p3/2 at 932.2 eV and S 2p3/2 at 161.8 eV corresponds to enargite but according to Mielczarski (1987) is also characteristic of cuprous sulphide (Cu2S). The fact that the relative proportions of both these elements are decreased to about one third of that found for fresh enargite suggests the presence of a partial surface layer, possibly composed in part of cuprous sulphide, occluding the mineral surface. However the ratio of Cu:As:S is approximately 9:3:12 which corresponds well to the stoichiometric ratio for enargite and does not support the presence of additional copper-containing compounds.
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
Fig. 5. Cu 2p, As 3d, S 2p, O 1s and C 1s high resolution photoelectron spectra recorded from the enargite electrode surface at 130 °C after application of +516 mV at pH 10 in a 103 M SEX solution. Table 3 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed on the enargite surface at 130 °C after application of +516 mV at pH 10 in a 103 M SEX solution.
Cu 2p3/2 Cu 2p1/2 O 1s O 1s OACAS C 1s CAC ref C 1s CAOAC S 2p3/2 sulphide S 2p1/2 sulphide S 2p3/2 EX S 2p1/2 EX As 3d5/2 surface As 3d3/2 surface As 3d5/2 bulk As 3d3/2 bulk
932.3 952.2 532.4 533.4 284.8 286.4 161.9 163.2 163.1 164.2 42.4 43.1 43.3 44.0
1.1 1.6 1.6 1.0 1.2 1.2 0.9 0.9 0.9 0.9 0.8 0.7 0.7 0.7
10.6 5.2 8.6 1.4 30.1 9.1 15.3 7.7 3.8 1.9 1.6 1.1 2.0 1.4
The presence of an O 1s peak at 531.2 eV is suggestive of Cu(OH)2 or possibly CuO, as a reduction product of the hydroxide form, according to Mielczarski (1987) and McIntyre and Cook (1975), although there is no evidence of any corresponding Cu (II) species. It therefore seems reasonable to conclude that the additional O 1s and C 1s species may represent residual decomposition products of xanthate remaining on the surface. Although only one S 2p species was detected, the BEs of S in enargite (Table 1) and S in xanthate (Table 2) vary by only about 0.2 eV,
so it is possible a second species is present but cannot be resolved. This can be conﬁrmed by examining the atomic ratio of Cu:As:S which, at 9.3:3.2:12.2 (Table 4), is very close to that of enargite (3:1:4). As there is no excess of sulphur, this is a strong indication the S 2p peak is from enargite alone. 3.4. Enargite in the presence of dithiophosphinate collector Adsorption of DTPI on chalcopyrite has been studied by Güler et al. (2006) using Diffuse Reﬂectance Fourier Transformation spectroscopy to determine the form of adsorbed collector species. They found that formation of cuprous-(DTPI) and dithiolate (a dimer of thiol, (DTPI)2) takes place as the predominant collector species on the surface, while adsorbed DTPI and a dithiophosphinate radical ((DTPI)0) was also detected in minor amounts on the mineral surface. The XPS results for enargite conditioned at +516 mV in the presence of DTPI are shown in Fig. 7 and the associated BEs are contained in Table 6, while the BE data for the bulk DTPI solution are presented in Table 5. It is evident from the XPS data that additional species are present on the enargite surface and that an incomplete surface layer exists, the former demonstrated by the presence of additional Cu, S and O species. The detection of Cu, As and S peaks at BEs corresponding to those seen for a fresh enargite surface, at signiﬁcantly reduced atomic concentrations, provide the evidence for the existence of a partially exposed mineral surface. In an atomic force microscopy (AFM) study of
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
Fig. 6. Cu 2p, As 3d, S 2p, O 1s and C 1s high resolution photoelectron spectra recorded from the enargite electrode surface at 130 °C after application of 400 mV at pH 10 in a 103 M SEX solution.
Table 4 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed on the enargite surface at 130 °C after application of 400 mV at pH 10 in a 103 M SEX solution.
Na 1s Cu 2p3/2 Cu 2p1/2 O 1s O 1s [email protected]
C 1s CAC ref C 1s CAO S 2p3/2 sulphide S 2p1/2 sulphide As 3d5/2 surface As 3d3/2 surface As 3d5/2 bulk As 3d3/2 bulk
1071.3 932.2 952.1 531.2 532.7 284.8 286.6 161.8 163.0 42.3 43.0 43.3 44.0
1.5 1.1 1.5 1.5 1.5 1.4 1.1 0.9 0.8 0.7 0.5 1.2 0.8
1.2 6.2 3.1 3.8 7.6 53.8 8.8 8.1 4.1 0.7 0.5 1.2 0.8
chalcopyrite and tennantite surfaces after treatment with the related DTP collector (Petrus et al., 2011a) the formation of so-called islands, composed of reaction products such as metal hydroxide species under alkaline conditions, was observed, indicating incomplete mineral surface coverage. Adhesion force measurement using AFM showed a decreasing trend after DTP treatment, and this increase in hydrophobicity was explained as a result of DTP adsorption.
The adsorption of DTPI is considered to take place by a chemisorption mechanism (Pecina-Treviño et al., 2003) and this mechanism has been further elaborated as consisting of a combination of chemical and electrochemical processes (Pecina et al., 2006) depending on the potential of the system. Where such a mechanism exists, reaction between the DTPI anion and the metal atoms exposed at the surface of the mineral lattice results in the formation of a metal–collector compound such as Pb(DTPI)2 in the case of galena (Pecina et al., 2006), and of Cu(DTPI) where chalcopyrite is involved (Güler et al., 2006). That such a mechanism also exists in the enargite-DTPI system is supported by the presence of the second Cu species (Cu 2p3/2 933.8 eV), in addition to the Cu in enargite (Cu 2p3/2 932.4 eV), detected by XPS and shown in Fig. 8. The presence of a second S 2p species in addition to that from the enargite, and a P 2p doublet, and to a lesser extent a C 1s peak at 286.0 eV, attributable to CAOAC bonding, based on the previous discussion, provide additional evidence for the presence of what is likely to be a Cu(DTPI) species. Further analysis of the surface after conditioning at 400 mV was necessary to conﬁrm the effects of treatment under conditions regarded as within the non-ﬂoating potential range for enargite, that is, at a potential below about 25 mV depending on system pH (Senior et al., 2006). The XPS spectra obtained from this surface are shown in Fig. 8 while the respective elemental binding energies are given in Table 7.
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
Fig. 7. Cu 2p, As 3d, S 2p, O 1s and C 1s high resolution photoelectron spectra recorded from the enargite electrode surface at 130 °C after application of +516 mV at pH 10 in a 103 M DTPI solution.
Table 5 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed in DTPI (Aerophine 3418A Promoter) at 130 °C.
Na 1s O 1s O 1s OACAS O 1s ex H2O C 1s CAC ref C 1s CAP S 2p3/2 S 2p1/2 P 2p3/2 P 2p1/2
1072.0 531.5 532.4 533.5 284.8 285.3 162.0 163.2 168.2 169.4
1.2 1.1 1.2 1.2 1.0 1.1 1.0 0.9 0.8 0.8
8.8 0.4 0.8 0.5 53.2 13.9 8.6 4.3 4.5 2.2
The Cu, As and S species detected correspond in their binding energies to those found in enargite, and no additional Cu species are present. No phosphorus was found on the surface and although a small amount of Na was found (about 3 atom%) this may be attributed to Na+ ions dissociated from DTPI in solution and deposited on the mineral surface. On its own it is not sufﬁcient evidence for the adsorption of collector on the surface. Additionally only one S 2p component is detected and with a S 2p3/2 BE of 161.5 eV, and this corresponds to sulphur in unaltered enargite where a BE of 161.8 eV was found.
Table 6 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed on the enargite surface at 130 °C after application of +516 mV at pH 10 in a 103 M DTPI solution.
Cu 2p3/2 I Cu 2p1/2 I Cu 2p3/2 II Cu 2p1/2 II O 1s O 1s C 1s CAC ref C 1s CAOAC S 2p3/2 S 2p1/2 S 2p3/2 S 2p1/2 As 3d5/2 (1) As 3d3/2 (1) As 3d5/2 (2) As 3d3/2 (2)
932.4 952.2 933.8 953.7 532.1 533.9 284.8 286.0 162.0 163.2 163.6 164.7 44.3 44.9 45.0 45.7
1.2 1.6 1.4 1.6 1.5 1.5 1.2 1.2 1.1 1.1 1.0 0.8 0.6 0.7 0.6 0.6
2.7 1.4 2.3 1.2 0.8 0.9 45.9 24.5 4.5 2.2 4.9 2.4 0.2 0.1 0.6 0.4
That collector adsorption is demonstrated at +516 but not at 400 mV suggests that in the case of the DTPI-enargite system an electrochemical–chemical mechanism as proposed by Pecina et al. (2006) is responsible for the interaction. Such a mechanism
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
Fig. 8. Cu 2p, As 3d, S 2p, O 1s and C 1s high resolution photoelectron spectra recorded from the enargite electrode surface at 130 °C after application of 400 mV at pH 10 in a 103 M DTPI solution.
Table 7 Binding energies, full width half-maxima and atomic concentrations of the elements identiﬁed on the enargite surface at 130 °C after application of 400 mV at pH 10 in a 103 M DTPI solution.
Na 1s Cu 2p3/2 Cu 2p1/2 O 1s O 1s O 1s CAO C 1s CAC ref C 1s CAOAC S 2p3/2 sulphide S 2p1/2 sulphide As 3d5/2 surface As 3d3/2 surface As 3d5/2 bulk As 3d3/2 bulk
1071.2 931.9 951.8 530.8 531.9 532.7 284.8 286.3 161.5 162.6 41.9 42.6 42.8 43.5
1.4 1.1 1.6 1.2 1.1 1.2 1.2 1.2 0.8 0.8 0.6 0.6 0.6 0.6
3.0 12.2 6.0 3.2 3.7 8.7 21.7 17.5 12.9 6.4 0.8 0.5 1.9 1.3
involves electrochemical oxidation of the mineral, followed by chemical formation of the metal–collector compound. 3.5. Mechanisms of collector adsorption Chemical mechanisms of adsorption of ﬂotation reagents on mineral surfaces include chemisorption, complexation, and chem-
ical adsorption. Chemisorption is a process where a chemical reaction takes place between the reagent, or adsorbate, and the surface, in the process creating new chemical bonds at the adsorbant surface. It has been argued (Buckley and Woods, 1997) that where thiol collectors interact with sulphide mineral surfaces, chemisorption is the thermodynamically favoured process. Other mechanisms of adsorption include electrostatic, which is a form of physical adsorption, and non-speciﬁc forces, such as Van der Waal’s or hydrogen bonding. According to Buckley and Woods (1997) the mechanism of attachment of thiol collectors to the mineral surface is electrochemical, and involves the anodic oxidation of the collector at the mineral surface together with a cathodic reaction, usually the reduction of oxygen. In an investigation of DTPI (Aerophine 3418A promoter) adsorption onto galena and pyrite (Pecina-Treviño et al., 2003; Pecina et al., 2006) three different mechanisms of adsorption are described, which depend on the mineral type and the conditions under which adsorption take place. Where the metal species shows chemical afﬁnity for the collector, a chemisorption process takes place. Where the potential is high enough to oxidise the mineral a two-step electrochemical–chemical process involving electrochemical oxidation of the mineral and chemical formation of a metal–collector compound is found. If the redox potential is sufﬁciently anodic to oxidise the collector then an electrochemical process of collector adsorption and dimer formation can occur.
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
These three mechanisms are in agreement with (Buckley and Woods, 1997) who found that anodic oxidation of thiol collectors, when it occurred at a sulphide mineral surface, can produce either a chemisorbed thiol, a metal collector compound, or a dithiolate, depending on the potential at which adsorption takes place. The effect of pre-oxidation of the sulphide mineral surface on the adsorption mechanism of thiol collectors was investigated using chalcocite and galena (Buckley et al., 2003), to determine if it caused a change in the collector species formed on the surface. It was found that the presence of metal oxide species made no difference, with the same collector species formed on the fresh and pre-oxidised surfaces. From this discussion the primary adsorption mechanism of thiol collectors on sulphide mineral surfaces is that of chemisorption, but the possible steps by which this adsorption process takes place depends on the potential of the system. A threshold potential (or potential range) for enargite ﬂoatability has been shown to exist, which implies collector adsorption does not occur at potentials sufﬁciently cathodic to prevent oxidation of the collector. Where enargite was conditioned at +516 mV in the presence of SEX, XPS suggests the formation of dixanthogen, which in the context of collector adsorption mechanisms discussed above, shows the potential is sufﬁciently anodic to oxidise the collector. Enargite is known to have poor ﬂoatability at cathodic potentials and the lack of any signiﬁcant evidence of collector after conditioning at 400 mV supports this ﬁnding. Where DTPI was used as the collector the species identiﬁed by XPS suggest the formation of a metal–collector compound, Cu(DTPI), similar to that found with chalcopyrite. Since the same anodic potential was used the implication is that DTPI is less subject to oxidation and adsorption takes place on the oxidised mineral surface.
3.6. Micro ﬂotation with pulp potential control Microﬂotation tests were conducted to conﬁrm the effects of conditioning at different redox potentials in the presence of collector on the ﬂotation recovery of enargite. Although many different variables have the potential to affect recovery, including Eh, collector type and dosage, ﬂotation time, gas rate, pH and others, the purpose of these tests was to conﬁrm the effects of conditioning at oxidising and reducing potentials in the presence of collector on hydrophobicity, therefore only the effects of Eh were investigated. Potentials of +500 and 400 mV were selected to correspond to anodic and cathodic peaks respectively identiﬁed in the CV studies, and also to ensure the test values were sufﬁciently separated from the transition potential range of approximately 100 to +100 mV to ensure the results were representative of ﬂotation in the ﬂoating or non-ﬂoating potential regions. An additional test was carried out at approximately +100 mV to evaluate ﬂotation performance in the region of the transition range, using SEX as the collector. However since automatic titrators were not used, maintaining precise control of Eh over a wide range of values was found to be impractical and no attempt was made to characterise ﬂotation recovery at closely spaced Eh values. Flotation recovery (as determined by mass recovery of enargite to the concentrate) using xanthate as the collector was found to be 82%, at +500 mV, at +100 mV 52% reported to the concentrate, and at 400 mV about 11% of the total sample mass was recovered. Using 3418A, a recovery of 69% was found at +500 mV, while at 400 mV this ﬁgure dropped to 31%. These results support the XPS ﬁndings where collector adsorption was conﬁrmed after conditioning at +516 mV but not 400 mV, and are also in agreement with published results, such as Smith and Bruckard (2007) and Bruckard et al. (2010), showing similar trends to these results.
3.7. General discussion Although this work demonstrates differences in collector adsorption according to potential, further study including investigation of whether collector adsorption at positive potentials is electrochemically reversible by subsequent application of cathodic potentials, is recommended to better characterise the nature of the adsorption mechanism. Development of a means of precise automatic pulp potential control in the UCT Micro Cell is also required to enable accurate determination of the transition potential range of enargite under different treatment conditions, particularly for different collectors. Investigation of alternative ﬂotation collectors with a high selectivity and strong afﬁnity for the arsenic sites in the enargite crystal structure is an essential step to facilitate an efﬁcient separation of arsenic-bearing sulphides from non-arsenic copper sulphides while minimising copper losses. Previous studies (Plackowski et al., 2014, 2013b) have focussed on the fundamental surface chemistry of enargite, in particular identiﬁcation of surface species formed as a result of applied potential. This work is not a ﬂotation study, but seeks to bridge the gap between previous fundamental work, and those investigations using pulp potential to control enargite ﬂotation (for example Bruckard et al., 2010; Smith and Bruckard, 2007). In this context the ﬂotation response has been used only to conﬁrm the effects of pulp potential on enargite ﬂoatability. Detailed ﬂotation studies to fully investigate the effects of Eh, collector type and dosage, as well as the effects of Eh on recovery in collectorless systems, although beyond the scope of this work, would add signiﬁcantly to our understanding of this complex system. Further ﬂotation work, in particular ﬂotation of mixed mineral systems, as well as investigation of mechanisms of collector adsorption on arsenicbearing sulphides, is necessary as the next step in achieving a commercially applicable selective ﬂotation process for arsenic mineral separation. Although use of pulp potential control has demonstrated that it is possible to achieve separation under idealised conditions, usually involving single mineral systems, typically separation efﬁciency is low and copper losses are high in more complex systems that attempt to replicate multi-mineral systems or conditions in an industrial ﬂotation plant. It has been shown that the ﬂotation response of a particular mineral, as found by single mineral studies, can be changed when another mineral type is present. Even in simple two-mineral systems, although single mineral studies predict separation can be achieved in a certain potential window, loss of selectivity in the combined system is signiﬁcant (Woods, 2003). In an industrial plant, the presence of multiple mineral types is likely to result in signiﬁcant loss of selectively. With careful process design it may be possible to overcome these limitations but the ﬂow sheet for such a process is complex, for example as proposed by Senior et al. (2006), likely to be difﬁcult to operate and speciﬁc to any given ore type. However, these factors must also be balanced against the increasing costs of treating high arsenic ores and the necessity of ﬁnding alternative treatment routes to enable processing of increasingly less favourable deposits as current reserves are depleted.
4. Conclusions Consideration has been given to the adsorption of SEX and DTPI onto the surface of natural enargite at pH 10 at applied potentials of 400 and +516 mV. Analysis of the results presented in this paper shows there is a signiﬁcant difference in the chemical composition on the surface of enargite after conditioning with the ﬂotation collectors at these potentials.
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73
XPS analysis shows that conditioning with xanthate at +516 mV results in the presence of C 1s and O 1s spectra diagnostic of xanthate adsorption, as well as BE differences in the S 2p combined with the presence of an additional S 2p spectrum after conditioning. Together these ﬁndings demonstrate the presence of xanthate on the enargite surface as a result of electrochemical treatment. After conditioning at 400 mV no evidence was found for xanthate adsorption with no additional S 2p species identiﬁed, and C 1s and O 1s species corresponding to adventitious hydrocarbon deposition detected. In addition, the Cu:As:S atom% ratio was in good agreement with the stoichiometrically correct ratio for enargite, showing no excess of sulphur or copper depletion. Investigation of the enargite/DTPI system also shows signiﬁcant differences in the surface speciation when the effects of these two different conditioning potentials are compared. After treatment at +516 mV additional Cu, S and O species to those in enargite alone exist on the surface and form an incomplete surface layer. While Cu, As and S peaks at BE’s corresponding to enargite are found, their signiﬁcantly reduced atomic concentrations support the argument for a mineral surface partially occluded by adsorbed collector. Similar to conditioning in the presence of xanthate at 400 mV, no evidence was found to conﬁrm the presence of DTPI species adsorbed on the enargite surface under these conditions. Floatability measurements using the UCT microﬂotation cell were used to assess the hydrophobicity of enargite mineral particles after conditioning at pulp potentials equivalent to the applied potentials used in the conditioning treatments for the XPS studies. The selected collectors were SEX and DTPI. Mass recovery of enargite was measured at potentials of +500, +100 and 400 mV. Using xanthate recovery, and therefore hydrophobicity, was greatest at high potential (82%), then decreased to 52% at +100 mV, while a poor ﬂotation response was observed at 400 mV with 11% mass recovery to concentrate. When DTPI was the collector, recoveries of 69% at high potential and 31% at low potential were recorded. These results were consistent with those of the XPS measurements of surface species present after conditioning at equivalent applied electrochemical potentials. Acknowledgments The authors gratefully acknowledge The University of Queensland (UQ) for an APA Scholarship (C.P.), CSIRO (Melbourne, Australia) for the top-up scholarship (C.P.) and research expenses support, Prof Dee Bradshaw from UQ for use of her UCT microﬂotation cell, and CMM (Centre for Microscopy and Microanalysis, UQ) for the facilities and assistance. References Bagci, E., Ekmekci, Z., Bradshaw, D., 2007. Adsorption behaviour of xanthate and dithiophosphinate from their mixtures on chalcopyrite. Miner. Eng. 20 (10), 1047–1053. Biswas, A.K., Davenport, W.G., 1994. Extractive metallurgy of copper, third ed. Pergamon, Oxford. Bradshaw, D.J., O’Connor, C.T., 1996. Measurement of the sub-process of bubble loading in ﬂotation. Miner. Eng. 9 (4), 443–448. Bruckard, W.J., Kyriakidis, I., Woodcock, J.T., 2007. The ﬂotation of metallic arsenic as a function of pH and pulp potential – a single mineral study. Int. J. Miner. Process. 84 (1–4), 25–32. Bruckard, W.J., Davey, K.J., Jorgensen, F.R.A., Wright, S., Brew, D.R.M., Haque, N., Vance, E.R., 2010. Development and evaluation of an early removal process for the beneﬁciation of arsenic-bearing copper ores. Miner. Eng. 23 (15), 1167– 1173. Buckley, A.N., Woods, R., 1997. Chemisorption—the thermodynamically favoured process in the interaction of thiol collectors with sulphide minerals. Int. J. Miner. Process. 51 (1–4), 15–26. Buckley, A.N., Goh, S.W., Lamb, R.N., Woods, R., 2003. Interaction of thiol collectors with pre-oxidised sulﬁde minerals. Int. J. Miner. Process. 72 (1–4), 163–174.
Castro, S.H., Baltierra, L., Hernandez, C., 2003. Redox conditions in the selective ﬂotation of enargite. In: Doyle, F.M., Woods, R. (Eds.), Proceedings – Electrochemical Society, The Electrochemical Society Inc., New Jersey, vol. 18., pp. 27–36. Chatterjee, A., Das, D., Mandal, B.K., Chowdhury, T.R., Samanta, G., Chakraborti, D., 1995. Arsenic in ground-water in 6 districts of West-Bengal, India – the biggest arsenic calamity in the world. 1. Arsenic species in drinking-water and urine of the affected people. Analyst 120 (3), 643–650. Cordova, R., Gomez, H., Real, S.G., Schrebler, R., Vilche, J.R., 1997. Characterization of natural enargite/aqueous solution systems by electrochemical techniques. J. Electrochem. Soc. 144 (8), 2628–2636. Fantauzzi, M., Atzei, D., Elsener, B., Lattanzi, P., Rossi, A., 2006. XPS and XAES analysis of copper, arsenic and sulfur chemical state in enargites. Surf. Interf. Anal. 38 (5), 922–930. Fornasiero, D., Fullston, D., Li, C., Ralston, J., 2001. Separation of enargite and tennantite from non-arsenic copper sulﬁde minerals by selective oxidation or dissolution. Int. J. Miner. Process. 61 (2), 109–119. Güler, T., Hiçyilmaz, C., Gökag˘aç, G., Ekmekçi, Z., 2004. Voltammetric and drift spectroscopy investigation in dithiophosphinate–chalcopyrite system. J. Colloid Interf. Sci. 279 (1), 46–54. Güler, T., Hiçyilmaz, C., Gökagaç, G., Ekmeçi, Z., 2006. Adsorption of dithiophosphate and dithiophosphinate on chalcopyrite. Miner. Eng. 19 (1), 62–71. Guo, H., 2004. Electrochemistry and ﬂotation of enargite and chalcopyrite. Doctor of Philosophy, Department of Mining Engineering, Queen’s University, Ontario, p. 270. Guo, H., Yen, W.T., 2002. Surface potential and wettability of enargite in potassium amyl xanthate solution. Miner. Eng. 15 (6), 405–414. Guo, H., Yen, W.T., 2005. Selective ﬂotation of enargite from chalcopyrite by electrochemical control. Miner. Eng. 18 (6), 605–612. Guo, H., Yen, W.T., 2006. Electrochemical ﬂoatability of enargite and effects of depressants. In: Önal, G., Acarkan, N., Çelik, M.S., Arslan, F., Atesßok, G., Güney, A., Sirkeci, A.A., Yüce, A.E., Perek, K.T. (Eds.), Proceedings of the XXIII International Mineral Processing Conference, Promed, Istanbul, Turkey, vol. 1, pp. 504–509. Guo, H., Yen, W.T., 2008. Electrochemical study of synthetic and natural enargites. In: Proceedings of [the] 24th International Mineral Processing Congress, Beijing, China, Sept. 24–28, 2008, vol. 1, pp. 1138–1145. Hampton, M.A., Plackowski, C., Nguyen, A.V., 2011. Physical and chemical analysis of elemental sulfur formation during galena surface oxidation. Langmuir 27 (7), 4190–4201. McIntyre, N.S., Cook, M.G., 1975. X-ray photoelectron studies on some oxides and hydroxides of cobalt, nickel, and copper. Anal. Chem. 47 (13), 2208–2213. Mielczarski, J., 1987. XPS study of ethyl xanthate adsorption on oxidized surface of cuprous sulﬁde. J. Colloid Interf. Sci. 120 (1), 201–209. Mielczarski, J.A., Cases, J.M., Alnot, M., Ehrhardt, J.J., 1996. XPS characterization of chalcopyrite, tetrahedrite, and tennantite surface products after different conditioning. 2. Amyl xanthate solution at pH 10. Langmuir 12 (10), 2531–2543. Pecina, E.T., Uribe, A., Finch, J.A., Nava, F., 2006. Mechanism of di-isobutyl dithiophosphinate adsorption onto galena and pyrite. Miner. Eng. 19 (9), 904– 911. Pecina-Treviño, E.T., Uribe-Salas, A., Nava-Alonso, F., Pérez-Garibay, R., 2003. On the sodium-diisobutyl dithiophosphinate (Aerophine 3418A) interaction with activated and unactivated galena and pyrite. Int. J. Miner. Process. 71 (1–4), 201–217. Petrus, H.T.B.M., Hirajima, T., Sasaki, K., Okamoto, H., 2011a. Effect of pH and diethyl dithiophosphate (DTP) treatment on chalcopyrite and tennantite surfaces observed using atomic force microscopy (AFM). Colloids Surf., A 389 (1–3), 266–273. Petrus, H.T.B.M., Hirajima, T., Sasaki, K., Okamoto, H., 2011b. Study of diethyl dithiophosphate adsorption on chalcopyrite and tennantite at varied pHs. J. Min. Sci. 47 (5), 695–702. Plackowski, C., Nguyen, A.V., Bruckard, W.J., 2012. A critical review of surface properties and selective ﬂotation of enargite in sulphide systems. Miner. Eng. 30, 1–11. Plackowski, C., Hampton, M.A., Nguyen, A.V., Bruckard, W.J., 2013a. The effects of Xray irradiation and temperature on the formation and stability of chemical species on enargite surfaces during XPS. Miner. Eng. 45 (5), 59–66. Plackowski, C., Hampton, M.A., Nguyen, A.V., Bruckard, W.J., 2013b. Fundamental studies of electrochemically controlled surface oxidation and hydrophobicity of natural enargite. Langmuir 29 (7), 2371–2386. Plackowski, C., Hampton, M.A., Bruckard, W.J., Nguyen, A.V., 2014. An XPS investigation of surface species formed by electrochemically induced surface oxidation of enargite in the oxidative potential range. Miner. Eng. 55 (1), 60–74. Ranta, L., Minni, E., Suoninen, E., Heimala, S., Hintikka, V., Saari, M., Rastas, J., 1981. XPS studies of adsorption of xanthate on sulﬁde surfaces. Appl. Surf. Sci. 7 (4), 393–401. Senior, G.D., Guy, P.J., Bruckard, W.J., 2006. The selective ﬂotation of enargite from other copper minerals – a single mineral study in relation to beneﬁciation of the Tampakan deposit in the Philippines. Int. J. Miner. Process. 81 (1), 15–26. Skinner, W.M., Prestidge, C.A., Smart, R.S.C., 1996. Irradiation effects during XPS studies of Cu(II) activation of zinc sulphide. Surf. Interf. Anal. 24 (9), 620–626. Smith, L.K., Bruckard, W.J., 2007. The separation of arsenic from copper in a Northparkes copper–gold ore using controlled-potential ﬂotation. Int. J. Miner. Process. 84 (1–4), 15–24.
C. Plackowski et al. / Minerals Engineering 65 (2014) 61–73 Valli, M., Persson, I., 1994. Interactions between sulphide minerals and alkylxanthates 8. A vibration and X-ray photoelectron spectroscopic study of the interaction between chalcopyrite, marcasite, pentlandite, pyrrhotite and troilite, and ethylxanthate and decylxanthate ions in aqueous solution. Colloids Surf., A 83 (3), 207–217. Velasquez, P., Ramos-Barrado, J.R., Cordova, R., Leinen, D., 2000. XPS analysis of an electrochemically modiﬁed electrode surface of natural enargite. Surf. Interf. Anal. 30 (1), 149–153.
Wittstock, G., Kartio, I., Hirsch, D., Kunze, S., Szargan, R., 1996. Oxidation of galena in acetate buffer investigated by atomic force microscopy and photoelectron spectroscopy. Langmuir 12 (23), 5709–5721. Woods, R., 2003. Electrochemical potential controlling ﬂotation. Int. J. Miner. Process. 72 (1–4), 151–162.